DOI: 10.17188/1476050
title: Materials Data on Sr3Ca5Fe4(CoO5)4 by Materials Project

description: Sr3Ca5Fe4(CoO5)4 crystallizes in the triclinic P1 space group. The structure is three-dimensional. there are twelve inequivalent Sr2+ sites. In the first Sr2+ site, Sr2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Sr–O bond distances ranging from 2.47–2.85 Å. In the second Sr2+ site, Sr2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Sr–O bond distances ranging from 2.42–2.95 Å. In the third Sr2+ site, Sr2+ is bonded in a 9-coordinate geometry to nine O2- atoms. There are a spread of Sr–O bond distances ranging from 2.45–3.17 Å. In the fourth Sr2+ site, Sr2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Sr–O bond distances ranging from 2.45–2.85 Å. In the fifth Sr2+ site, Sr2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Sr–O bond distances ranging from 2.44–2.91 Å. In the sixth Sr2+ site, Sr2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Sr–O bond distances ranging from 2.44–2.90 Å. In the seventh Sr2+ site, Sr2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Sr–O bond distances ranging from 2.43–2.86 Å. In the eighth Sr2+ site, Sr2+ is bonded in a 9-coordinate geometry to nine O2- atoms. There are a spread of Sr–O bond distances ranging from 2.48–3.17 Å. In the ninth Sr2+ site, Sr2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Sr–O bond distances ranging from 2.49–2.81 Å. In the tenth Sr2+ site, Sr2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Sr–O bond distances ranging from 2.45–2.84 Å. In the eleventh Sr2+ site, Sr2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Sr–O bond distances ranging from 2.45–2.91 Å. In the twelfth Sr2+ site, Sr2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Sr–O bond distances ranging from 2.43–2.83 Å. There are twenty inequivalent Ca2+ sites. In the first Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.34–2.91 Å. In the second Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.34–2.89 Å. In the third Ca2+ site, Ca2+ is bonded in a 7-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.34–2.98 Å. In the fourth Ca2+ site, Ca2+ is bonded in a 7-coordinate geometry to seven O2- atoms. There are a spread of Ca–O bond distances ranging from 2.32–2.57 Å. In the fifth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.30–2.91 Å. In the sixth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.38–2.85 Å. In the seventh Ca2+ site, Ca2+ is bonded in a 7-coordinate geometry to seven O2- atoms. There are a spread of Ca–O bond distances ranging from 2.35–2.59 Å. In the eighth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.37–2.89 Å. In the ninth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.35–2.90 Å. In the tenth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.31–2.93 Å. In the eleventh Ca2+ site, Ca2+ is bonded in a 7-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.32–2.97 Å. In the twelfth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.31–2.96 Å. In the thirteenth Ca2+ site, Ca2+ is bonded in a 7-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.30–2.98 Å. In the fourteenth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.35–2.95 Å. In the fifteenth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.35–2.80 Å. In the sixteenth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.34–2.84 Å. In the seventeenth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.34–2.99 Å. In the eighteenth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.36–2.97 Å. In the nineteenth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.36–2.96 Å. In the twentieth Ca2+ site, Ca2+ is bonded in a 7-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.35–3.00 Å. There are sixteen inequivalent Fe3+ sites. In the first Fe3+ site, Fe3+ is bonded to four O2- atoms to form FeO4 tetrahedra that share corners with two CoO6 octahedra and corners with two FeO4 tetrahedra. The corner-sharing octahedra tilt angles range from 34–41°. There are a spread of Fe–O bond distances ranging from 1.86–1.95 Å. In the second Fe3+ site, Fe3+ is bonded to four O2- atoms to form FeO4 tetrahedra that share corners with two CoO6 octahedra and corners with two FeO4 tetrahedra. The corner-sharing octahedra tilt angles range from 32–34°. There are a spread of Fe–O bond distances ranging from 1.86–1.95 Å. In the third Fe3+ site, Fe3+ is bonded to four O2- atoms to form FeO4 tetrahedra that share corners with two CoO6 octahedra and corners with two FeO4 tetrahedra. The corner-sharing octahedra tilt angles range from 33–39°. There are a spread of Fe–O bond distances ranging from 1.86–1.97 Å. In the fourth Fe3+ site, Fe3+ is bonded to four O2- atoms to form FeO4 tetrahedra that share corners with two CoO6 octahedra and corners with two FeO4 tetrahedra. The corner-sharing octahedra tilt angles range from 28–37°. There are a spread of Fe–O bond distances ranging from 1.88–1.96 Å. In the fifth Fe3+ site, Fe3+ is bonded to four O2- atoms to form FeO4 tetrahedra that share corners with two CoO6 octahedra and corners with two FeO4 tetrahedra. The corner-sharing octahedra tilt angles range from 33–39°. There are a spread of Fe–O bond distances ranging from 1.86–1.97 Å. In the sixth Fe3+ site, Fe3+ is bonded to four O2- atoms to form FeO4 tetrahedra that share corners with two CoO6 octahedra and corners with two FeO4 tetrahedra. The corner-sharing octahedra tilt angles range from 32–36°. There are a spread of Fe–O bond distances ranging from 1.88–1.95 Å. In the seventh Fe3+ site, Fe3+ is bonded to four O2- atoms to form FeO4 tetrahedra that share corners with two CoO6 octahedra and corners with two FeO4 tetrahedra. The corner-sharing octahedra tilt angles range from 36–41°. There are a spread of Fe–O bond distances ranging from 1.86–1.96 Å. In the eighth Fe3+ site, Fe3+ is bonded to four O2- atoms to form FeO4 tetrahedra that share corners with two CoO6 octahedra and corners with two FeO4 tetrahedra. The corner-sharing octahedra tilt angles range from 32–39°. There are a spread of Fe–O bond distances ranging from 1.87–1.95 Å. In the ninth Fe3+ site, Fe3+ is bonded to four O2- atoms to form FeO4 tetrahedra that share corners with two CoO6 octahedra and corners with two FeO4 tetrahedra. The corner-sharing octahedra tilt angles range from 37–41°. There are a spread of Fe–O bond distances ranging from 1.86–1.95 Å. In the tenth Fe3+ site, Fe3+ is bonded to four O2- atoms to form FeO4 tetrahedra that share corners with two CoO6 octahedra and corners with two FeO4 tetrahedra. The corner-sharing octahedral tilt angles are 34°. There are a spread of Fe–O bond distances ranging from 1.86–1.95 Å. In the eleventh Fe3+ site, Fe3+ is bonded to four O2- atoms to form FeO4 tetrahedra that share corners with two CoO6 octahedra and corners with two FeO4 tetrahedra. The corner-sharing octahedra tilt angles range from 37–38°. There are a spread of Fe–O bond distances ranging from 1.86–1.95 Å. In the twelfth Fe3+ site, Fe3+ is bonded to four O2- atoms to form FeO4 tetrahedra that share corners with two CoO6 octahedra and corners with two FeO4 tetrahedra. The corner-sharing octahedra tilt angles range from 31–36°. There are a spread of Fe–O bond distances ranging from 1.88–1.96 Å. In the thirteenth Fe3+ site, Fe3+ is bonded to four O2- atoms to form FeO4 tetrahedra that share corners with two CoO6 octahedra and corners with two FeO4 tetrahedra. The corner-sharing octahedra tilt angles range from 34–41°. There are a spread of Fe–O bond distances ranging from 1.87–1.96 Å. In the fourteenth Fe3+ site, Fe3+ is bonded to four O2- atoms to form FeO4 tetrahedra that share corners with two CoO6 octahedra and corners with two FeO4 tetrahedra. The corner-sharing octahedra tilt angles range from 28–36°. There are a spread of Fe–O bond distances ranging from 1.85–1.95 Å. In the fifteenth Fe3+ site, Fe3+ is bonded to four O2- atoms to form FeO4 tetrahedra that share corners with two CoO6 octahedra and corners with two FeO4 tetrahedra. The corner-sharing octahedra tilt angles range from 34–39°. There are a spread of Fe–O bond distances ranging from 1.86–1.96 Å. In the sixteenth Fe3+ site, Fe3+ is bonded to four O2- atoms to form FeO4 tetrahedra that share corners with two CoO6 octahedra and corners with two FeO4 tetrahedra. The corner-sharing octahedra tilt angles range from 29–35°. There are a spread of Fe–O bond distances ranging from 1.87–1.97 Å. There are sixteen inequivalent Co3+ sites. In the first Co3+ site, Co3+ is bonded to six O2- atoms to form CoO6 octahedra that share corners with four CoO6 octahedra and corners with two FeO4 tetrahedra. The corner-sharing octahedra tilt angles range from 11–12°. There are a spread of Co–O bond distances ranging from 1.93–2.22 Å. In the second Co3+ site, Co3+ is bonded to six O2- atoms to form CoO6 octahedra that share corners with four CoO6 octahedra and corners with two FeO4 tetrahedra. The corner-sharing octahedra tilt angles range from 6–9°. There are a spread of Co–O bond distances ranging from 1.86–2.28 Å. In the third Co3+ site, Co3+ is bonded to six O2- atoms to form CoO6 octahedra that share corners with four CoO6 octahedra and corners with two FeO4 tetrahedra. The corner-sharing octahedra tilt angles range from 10–15°. There are a spread of Co–O bond distances ranging from 1.95–2.21 Å. In the fourth Co3+ site, Co3+ is bonded to six O2- atoms to form CoO6 octahedra that share corners with four CoO6 octahedra and corners with two FeO4 tetrahedra. The corner-sharing octahedra tilt angles range from 7–11°. There are a spread of Co–O bond distances ranging from 1.86–2.31 Å. In the fifth Co3+ site, Co3+ is bonded to six O2- atoms to form CoO6 octahedra that share corners with four CoO6 octahedra and corners with two FeO4 tetrahedra. The corner-sharing octahedra tilt angles range from 11–13°. There are a spread of Co–O bond distances ranging from 1.94–2.24 Å. In the sixth Co3+ site, Co3+ is bonded to six O2- atoms to form CoO6 octahedra that share corners with four CoO6 octahedra and corners with two FeO4 tetrahedra. The corner-sharing octahedra tilt angles range from 9–11°. There are a spread of Co–O bond distances ranging from 1.85–2.21 Å. In the seventh Co3+ site, Co3+ is bonded to six O2- atoms to form CoO6 octahedra that share corners with four CoO6 octahedra and corners with two FeO4 tetrahedra. The corner-sharing octahedra tilt angles range from 10–14°. There are a spread of Co–O bond distances ranging from 1.95–2.19 Å. In the eighth Co3+ site, Co3+ is bonded to six O2- atoms to form